lattice and electron
phonon coupling in 3
Kenneth R. O’Neal 1, Arpita Paul2, Amal al-Wahish1,3,4, Kendall D. Hughey1, Avery L. Blockmon1, Xuan Luo5,6,7, Sang-Wook Cheong5,6,8, Vivien S. Zapf 9, Craig V. Topping10, John Singleton 9, Mykhalo Ozerov 11, Turan Birol 12and Janice L. Musfeldt 1,13
While 3d-containing materials display strong electron correlations, narrow band widths, and robust magnetism, 5dsystems are recognized for strong spin–orbit coupling, increased hybridization, and more diffuse orbitals. Combining these properties leads to novel behavior. Sr3NiIrO6, for example, displays complex magnetism and ultra-high coerciveﬁelds—up to an incredible 55 T. Here,
we combine infrared and optical spectroscopies with high-ﬁeld magnetization andﬁrst-principles calculations to explore the fundamental excitations of the lattice and related coupling processes including spin–lattice and electron–phonon mechanisms. Magneto-infrared spectroscopy reveals spin–lattice coupling of three phonons that modulate the Ir environment to reduce the energy required to modify the spin arrangement. While these modes primarily affect exchange within the chains, analysis also uncovers important inter-chain motion. This provides a mechanism by which inter-chain interactions can occur in the developing model for ultra-high coercivity. At the same time, analysis of the on-site Ir4+excitations reveals vibronic coupling and extremely large crystalﬁeld parameters that lead to at2g-derived low-spin state for Ir. Theseﬁndings highlight the spin–charge–lattice
entanglement in Sr3NiIrO6and suggest that similar interactions may take place in other 3d/5dhybrids.
npj Quantum Materials (2019) 4:48 ; https://doi.org/10.1038/s41535-019-0184-x
Interest in 5d materials and 3d/5d hybrids has blossomed in response to recent scientiﬁc advances and applications in hard magnets, topological insulators, multiferroics, superconductors, and thermoelectrics.1–6 5d materials are unique for several
reasons. First, strong spin–orbit coupling competes with magnetic, crystal-ﬁeld, many-body Coulomb, and other interactions to drive new physical behaviors,7 such as the J
eff=1/2 state in certain
iridates.8,9Second, the bonding interactions associated with the larger 5d orbitals promote inter-cation dimerization in pairwise, chain-like, and other complex orderings.10,11Third, the relativistic shifts in orbital energies, combined with spin–orbit and band-width effects, can drive band inversions leading to topological phases and enhanced Rashba splittings.12–15 In contrast, 3d transition metal compounds typically display much narrower bandwidths, more robust magnetism, and stronger electron–electron interactions, and correlations.16,17 When these two sets of properties are brought together, as in Sr3NiIrO6, new
and potentially useful behaviors can emerge.
What makes Sr3NiIrO6 so remarkable is the extraordinary
coercivity—up to 55 T depending on sample details.18By contrast, traditional hard magnets like Fe/Pt, Nd31−xDyxFebalCo2B1(x=7 wt %),
and LuFe2O4 have coercivities on the order of 1, 3, and 9 T,
respectively.19–21The extraordinarily high coerciveﬁeld is not due
to ferromagnetic domains since the material is antiferromagnetic, though the exact mechanism remains to be understood.18,22–24
The crystal structure consists of chains of alternating face-sharing NiO6trigonal prisms and IrO6octahedra stacked along the c axis with Sr atoms separating the chains. These chains are arranged in a triangular conﬁguration in theabplane.25Because Ir has a 4+ charge, it was originally thought to have a Jeff=1/
2 state.23,26,27A trigonal distortion, however, breaks the symmetry and creates a slight deviation from the pureJeff=1/2.
is part of a chemical family of quasi-one-dimensional 3d/5d hybrids with formula A3BB′O6. Notably, these materials display
increasing coercive magneticﬁelds as theB′site ion evolves from a 3dto a 4dto a 5dmagnetic ion.18,25,29 This suggests that the unusual properties of Ir and similar 5dions must play an important role in creating the high coercivity. Recent calculations indeed suggest that it is the strongly anisotropic exchange interaction characteristic of the Ir4+ ion that plays a key role in the high coercive magnetic ﬁeld.24 The strongest magnetic exchange is antiferromagnetic between Ni and Ir ions within c axis chains, which creates one-dimensional order below ≈200 K.27 Elastic neutron diffraction measurements identiﬁed two potential mag-netic ground states at zeroﬁeld: a partially disordered antiferro-magnet or a more complex, spatially modulated state.26In light of the large Ni···Ir intra-chain exchange interactions,27 the partially
Received: 1 May 2019 Accepted: 22 July 2019
Department of Chemistry, University of Tennessee, Knoxville, TN 37996, USA;2
Department of Chemical Engineering and Materials Science, University of Minnesota, Minneapolis, MN 55455, USA;3
Department of Physics, University of Washington, Seattle, WA 98105, USA;4
Department of Physics, Seattle University, Seattle, WA 98122, USA;5
Max Planck POSTECH/Korea Research Initiative, Pohang University of Science and Technology, Pohang 37673, Korea;6
Laboratory for Pohang Emergent Materials, Pohang Accelerator Laboratory, Pohang 37673, Korea;7Key Laboratory of Materials Physics, Institute of Solid State Physics, Chinese Academy of Sciences, 230031 Hefei, China;8Rutgers Center for Emergent Materials and Department of Physics and Astronomy, Rutgers University, Piscataway, NJ 08854, USA;9
National High Magnetic Field Laboratory, MS E536, Los Alamos National Laboratory, Los Alamos, NM 87545, USA;10School of Physics & Astronomy, University of St Andrews, North Haugh, St Andrews KY16 9SS, UK;11National High Magnetic Field Laboratory, Tallahassee, FL 32310, USA;12
Chemical Engineering and Materials Science, University of Minnesota, Minneapolis, MN 55455, USA and13
Department of Physics and Astronomy, University of Tennessee, Knoxville, TN 37996, USA
disordered antiferromagnet model is most likely and has been suggested for severalA3BB′O6materials with high coerciveﬁeld.
In this model, caxis chains act like giant spin units due to the difference between the Ni and Ir moments, with frustrated antiferromagnetic interactions between chains in the ab plane. Consequently, the ground state consists of two oppositely aligned chains and one with random orientation. In this model, gradual
ﬂipping of the randomly oriented third chains accounts for the spin glass-like dynamics with magnetic hysteresis and coercivity that is seen below 15 K in Sr3NiIrO6and for the initial evolution of
the magnetization up to the coerciveﬁeld. At the coerciveﬁeld, the second chain ﬂips, leading to a sudden jump and the high coerciveﬁeld. The extraordinary coercivity must result from the barrier to ﬂipping of the second chain due to its many-body nature and interactions with the lattice including the anisotropic exchange interaction of Ir. Thus, if we are to achieve a complete understanding of the extraordinary coercive magnetic ﬁeld in Sr3NiIrO6, we need to quantify how the magnetic order and Ir
electronic state interact with the lattice.
To this end, we measured the infrared and optical properties of Sr3NiIrO6and compared the response to high-ﬁeld magnetization,
ﬁrst-principles lattice dynamics calculations, and simulations of spin–phonon coupling. While the phonons are nearly rigid across the magnetic ordering and freezing transitions, magneto-infrared work reveals three modes that track the magnetic response. What distinguishes these modes is how they modulate superexchange pathways around the Ir centers. The O-Ir-O bending mode near 310 cm−1 is the dominant feature with an exceptionally large spin–lattice coupling constant—on the order of 10 cm−1. That
very speciﬁc local lattice distortions are involved in the approach to the coerciveﬁeld provides further conﬁrmation that the
high-ﬁeld transition in Sr3NiIrO6 is more than a simple domain
reorientation process.18 At the same time, we reached beyond
spin–lattice interactions to explore electron–phonon coupling. Analysis of the Ir4+on-sited-to-dexcitations reveals that they are vibronically activated. An oscillator strength analysis uncovers electron–phonon coupling involving the 177 cm−1 Ni in-plane
mode, which modulates the Ni-O-Ir bond angles (and thus the local Ir4+environments). We discuss these ﬁndings in terms of inter- and intra-chain coupling as well as how the diffuse character of the Ir 5dorbitals enlarges the crystalﬁeld parameters to give a spin conﬁguration that stems from thet2g-derived energy levels.
RESULTS AND DISCUSSION
Strong spin–lattice coupling and intra-chain interactions in Sr3NiIrO6
Figure1a displays the infrared spectrum of Sr3NiIrO6. A symmetry
analysis of theR3cspace group yields 7 A2uand 12 Eu
infrared-active phonons—consistent with our spectra. Our mode assign-ments are based on lattice dynamics calculations, which also provide symmetries and displacement patterns. These assign-ments are summarized in Table S1 (Supplementary Information) and allow the microscopic interactions indicated by the spectra to be fully understood. Spin–lattice coupling across the 75 K magnetic ordering and 15 K freezing temperatures is extremely weak (Supplementary Information), likely because these energy scales do not correspond to collective transitions.18,25,26 The signature in other thermodynamic probes is not strong either. Magnetoelastic coupling in appliedﬁeld, however, is robust.
In order to search for elastic contributions to the record high coercivity, we measured the magneto-infrared response of Sr3NiIrO6 (Fig. 1). Here, magnetic ﬁeld was increased step-wise
from 0 to 35 T, and spectra were acquired at each step to avoid complications from magnetic hysteresis. The measurements therefore follow the line from the origin in Fig.1b, shown more closely in Fig.1c. The absorption difference (Δα=α(30 T)−α(0 T))
in the upper portion of Fig. 1a highlights spectral differences. Three phonons are sensitive to magneticﬁeld. The Eusymmetry
mode at 310 cm−1displays the largest magneto-infrared response (Fig.1f). The A2usymmetry modes at 133 and 534 cm−
are also sensitive to changes in the microscopic spin arrangement (Fig.1d, h). Interestingly, the two lower frequency phonons harden with appliedﬁeld, whereas the higher frequency mode softens.
We quantify the magnetic ﬁeld dependence of the 133, 310, and 534 cm−1phonons by integrating the absolute value of the absorption difference over a narrow frequency window (Rω2
ω1jΔαjdω) at each ﬁeld. This quantity is proportional to the ﬁeld-induced frequency shift, although error bars onΔαare much smaller.33 Comparison with the bulk magnetization (Fig. 1c) reveals that these changes grow as magnetization squared.34This implies that the ﬁeld-driven transition is not just a spin reorientation process; it also involves speciﬁc local lattice distortions. The magnetic ﬁeld drives the spin rearrangement, while cooperative lattice distortions reduce the exchange inter-actions and the energy required to modify the microscopic spin arrangement. Similar mechanisms are active in other materials.34–36
While the 48 T spin-reorientationﬁeld is beyond the current reach of resistive magnets, the observed spin–phonon coupling is quite strong. We can estimate the spin–phonon coupling constants in Sr3NiIrO6asω=ω0+λ〈Si·Sj〉. Here, ω0 is the unperturbed (zero
ﬁeld) mode frequency, ω is the perturbed (high ﬁeld) mode frequency, and 〈Si·Sj〉 is the spin–spin correlation function.37
Taking the limiting low temperature value of the spin–spin correlation function as <SiSj>¼<112>¼12, we ﬁnd λ≈2, 10,
and 5 cm−1for the 133, 310, and 534 cm−1modes, respectively. By comparison, the highest value ofλin the 3d/4phybrid Ni3TeO6at
the same applied magnetic ﬁeld (i.e., across the spin–ﬂop transition) is 4 cm−1.38This suggests that higherﬁelds may drive even stronger spin–lattice interactions, especially across the coerciveﬁeld.39,40
Examination of the calculated displacement patterns uncovers important similarities in the spin–lattice coupled modes that provide mechanistic insight into the ﬁeld-driven process. The Eu
symmetry O-Ir-O bending mode at 310 cm−1is the most sensitive to ﬁeld (Fig. 1g). This displacement pattern—with its strong O component—unambiguously modulates the superexchange inter-actions between Ir and its neighbors by changing the Ir environment. This motion also reduces the symmetry of the crystal and (as discussed below) introduces new terms into the magnetic Hamiltonian. Local lattice distortions of this type are thus important to the development of various spin rearrange-ments—such as that across the coercive ﬁeld. The other two magneto-infrared-active features modulate the exchange interac-tions around the Ir centers as well—although by less effective routes. For instance, the A2usymmetry mode at 133 cm−1consists
of Sr out-of-plane displacement and in-phase Ni displacement along thecaxis (Fig.1e) that slightly varies the Ni-O-Ir angle as a second-order effect. The A2usymmetry mode at 534 cm−1, on the
other hand, consists mainly of O stretching around the Ir center (Fig. 1i), which also impacts the superexchange angles. The aforementioned displacement patterns primarily affect exchange within the chains. A view along the chains (see animations of the displacement patterns in Supplementary Information) reveals that these modes have inter-chain motion as well. This supports the role of inter-chain interactions in the developing magnetic model18,26 and provides a mechanism by which such effects can occur.
The form of the spin–phonon Hamiltonian for Sr3NiIrO6is very
complicated—even when considering only intra-chain interac-tions—because various phonons break lattice symmetries and allow novel magnetic interaction terms (such as Dzyaloshinskii–Moriya) to emerge (see the Supplementary Infor-mation for details). This makes the ﬁrst-principles calculation of every spin–phonon coupling parameter practically impossible. We 2
therefore developed a simpliﬁed approach to predict which phonon modes have a stronger effect on the magnetic structure (and vice versa). We began by considering the displacement pattern of the 310 cm−1 mode and calculated the effect of this type of modulation on the ground-state spin arrangement. Similar calculations using the 177 cm−1 mode pattern are included for comparison. As a reminder, the Eusymmetry O-Ir-O bending mode
at 310 cm−1engages in spin–lattice coupling, whereas (as we shall see below) the Eusymmetry mode at 177 cm−
is the phonon that vibronically activates on-sited-to-d excitations of Ir4+. When the atoms are not displaced, the Ni and Ir moments are predicted to be collinear and parallel to thecaxis (within error bars), consistent with the observed magnetism. Displacing atoms according to the pattern of the 310 cm−1mode leads to very signiﬁcant tilting of
the Ni spin moment as well as weaker tilting of the Ir spin (Fig.1j). As a result, the system becomes non-collinear. The 177 cm−1 mode, on the other hand, leads to a much smaller effect on the magnetic structure, in line with a lack ofﬁeld-induced changes of this mode. This reveals the complex nature of the spin–lattice coupling and suggests that the induced tilting may lower the magnetic switching barrier.
Electron–phonon coupling and strength of the crystalﬁeld interactions in Sr3NiIrO6
Equipped with a microscopic understanding of the elastic distortions in response to the magnetic ﬁeld, we sought to determine whether similar phonons contribute to the electronic
0.0 0.1 0.2 0.3 0.4 0.5
0 2 4 6 8 10 12
Total Displacement (Å)
Ni(310 cm -1
Ir(310 cm -1
Ni(177 cm -1
Ir(177 cm -1
530 540 550
-25 0 25 50 75 100 125
3 T 9 T 15 T 21 T 27 T 30 T
280 300 320 340
0 100 200 300
5 T 10 T 15 T 20 T 25 T 30 T
110 120 130 140 150 160
0 50 100 150
)5 T 10 T 15 T 20 T 25 T 30 T 35 T 100 200 300 400 500 600 0
500 1000 1500 2000
30 T 0 T
-200 -150 -100 -50 0 50
0 10 20 30 40
0.0 0.1 0.2 0.3 0.4 0.5
2 , and
Magnetic Field (T)
0 10 20 30
0.00 0.05 0.10
-60 -40 -20 0 20 40 60 -10
-5 0 5 10
-26.2 T 29.6 T
Sample moment (Arb. Units)
Magnetic Field (T) 48.4 T
φ φ φ
Fig. 1 Magnetoelastic coupling in Sr3NiIrO6.aAbsorption of polycrystalline Sr3NiIrO6at 0 and 30 T at 4.2 K. The high-ﬁeld spectrum is offset for clarity. Top portion displays the 30 Tﬁeld-induced absorption difference. Vertical gray bands highlight changes.bHysteresis loop of polycrystalline Sr3NiIrO6at 4.0 K. The indicated criticalﬁelds for spin rearrangements are not as high as single crystal measurements due to an averaged response of different orientations.cMagnetization, square of the magnetization, and integrated absorption differences for the three features of interest versus magneticﬁeld. Values are normalized at fullﬁeld for comparison, and a representative error bar (standard deviation) is shown. The inset is a close-up view of the same data.d,f,hClose-up views of the absorption difference spectra in the regions of interest and their development with magneticﬁeld. Curves are offset for clarity. e,g,iCalculated phonon displacement patterns for theseﬁ eld-sensitive modes.jFirst-principles simulation of spin–lattice coupling-induced canting of the Ni and Ir spin moments with respect to thecaxis as a function of ionic displacement chosen to mimic the 310 and 177 cm−1mode patterns. The magnitude of the displacement is given for a total of 22 atoms in the unit cell (which has two formula units)
properties—speciﬁcally the vibronically activated crystal ﬁeld excitations of Ir4+. The Ir4+electronic conﬁguration is the key to
creating the anisotropic exchange interactions that have been identiﬁed as an important contributor to the high coerciveﬁeld, suggesting that additional insight would prove useful. We therefore measured the optical properties of Sr3NiIrO6as well as
the Cu analog, Sr3CuIrO6, to track the Ir4+on-site excitations near
0.7 eV (Fig.2a and Supplementary Information). While the position and general behavior of these excitations agree with prior resonant inelastic x-ray scattering work,28,41 our measurements offer signiﬁcantly higher spectral resolution. The presence of intra-t2g on-site excitations indicates that the Ir4+ site symmetry is
slightly distorted from octahedral, creating a distortion away from a pure Jeff=1/2 state.28 Moreover, analysis reveals that these
excitations are vibronically activated by a phonon that is distinct from those that contribute to the coercivity via spin–lattice pathways.
Inter-band excitations, like those in Sr3NiIrO6, are responsible for
the colors of transition metal-containing materials and have been extensively studied.42–44Vibronic coupling, in which an odd-parity
phonon mixes with a d-to-d excitation, is a common activation mechanism.42–44 Here, both spin and parity selection rules are broken due to coupling with a phonon. In this scenario, the temperature dependence of the oscillator strength is modeled as f=fx+f0coth(hν/2kBT), whereνis the frequency of the activating
phonon; f0 is the oscillator strength at base temperature; fx
represents oscillator strength from other mixing processes; andh, kB, andThave their usual meanings.45This model can be used to
determine which phonon activates the electronic transition. While phonon-assisted d-to-d excitations have been reported in Sr3Ir2O7,46 quantitative vibronic coupling analyses (such as we
do here) are rare in 4dand 5dsystems, and particularly so in 3d/5d hybrids.
Figure2b displays the oscillator strength analysis of the Ir4+
on-site excitations in Sr3NiIrO6. There is a small deviation from the
overall trend near 70 K that may be due to the spin ordering transition,47 but the size of our error bars precludes a detailed analysis. Examination reveals that the Ir-relatedd-to-dexcitations are vibronically coupled with the 177 cm−1Euphonon—which is
present in the infrared spectrum (Fig. 2c). According to our calculations, this mode consists of Ni in-plane motion against Sr counter-motion that indirectly modulates the Ir environment (Fig. 2d). Thus, the vibronically coupled mode is separate and distinct from those involved in magnetoelastic coupling (133, 310, and 534 cm−1). This separation offers the possibility of selective property control. We also carried out the same analysis for the more distorted Cu analog and unveiled coupling to a different displacement in which O motion more directly affects the Ir environment (Supplementary Information). This contrast likely emanates from the dissimilar chain conﬁgurations (linear for the Ni system and zigzag for the Cu analog), highlighting the importance of local symmetry in coupling processes.
The observation of Ir4+ excitations offers an opportunity to
compare crystal ﬁeld parameters of a 5d center to the more commonly studied 3d-containing oxides. Based on the position and shape of the Ir-related intra-band excitations of Sr3NiIrO6
and the d5 Tanabe–Sugano diagram,48–50 we estimate 10Dq= 3.24 eV and the Racah parameterB=1.18 eV. As a reminder, 10Dq and B describe the strength of crystal ﬁeld interactions, and because 5dorbitals are highly diffuse, the crystalﬁeld parameters are large. Weﬁnd 10Dq=2.33 eV andB=0.86 eV for Sr3CuIrO6.41
As summarized in Table 1, these values are similar to other Ir4+-containing materials, including Sr2IrO4 and Li2IrO3,51–53 but
much higher than prototypical transition metal oxides like α -Fe2O354 and even the 3d/4p hybrid Ni3TeO6.55 We attribute this
difference to the heavy mass of the Ir center, which is predicted to 150 200 250
200 400 600 800
Frequency (cm-1) 177 cm-1
0.4 0.6 0.8 1.0
500 1000 1500
0 100 200 300
2.4 2.6 2.8 3.0 3.2 3.4
f = fx+f0coth(hν/2kT)
fx= 1.86x10-6 f0= 5.68x10-7 ν=178cm-1
Fig. 2 Vibronic coupling of Ir4+excitations in Sr3NiIrO6.aOptical absorption of Sr3NiIrO6in the vicinity of the Ir4+on-site excitations at select
temperatures.bOscillator strength analysis using the indicated vibronic coupling model, whereνis the coupled phonon frequency.cThe infrared spectrum shows phonons near the extractedνvalue.dCalculated displacement pattern for the vibronically coupled phonon
Table 1. Vibronic coupling and crystalﬁeld parameters
Material Element Electronic state 10Dq(eV) B(eV) Coupled phonon frequency (cm−1) Displacement Refs.
Sr3NiIrO6 Ir 5d5 3.24 1.18 177 Ni in-plane motion This work
Sr3CuIrO6 Ir 5d5 2.33 0.86 273 O-Ir-O bend This work
Sr2IrO4 Ir 5d5 3.8 0.93 – – 48,49
Li2IrO3 Ir 5d5 2.7 0.95 – – 50
Ni3TeO6 Ni 3d8 1.10 0.11 – – 51
α-Fe2O3 Fe 3d5 1.59 0.09 525 In-plane, in-phase Fe-O stretch 52,53
Summary of 10Dqand Racah parameters for the 3d/5dmaterials in this study compared to the crystalﬁeld parameters of other Ir-containing compounds along with information about the vibronically coupled phonons. No vibronic coupling analysis was found for Sr2IrO4or Li2IrO3, and the Ni2+excitations in
Ni3TeO6are not vibronically activated, so no phonons are implicated
increase spin–orbit coupling and Racah parameters in free ions.56
Importantly, the large 10Dqvalues separate thet2gand eglevels
such that the eg-derived bands in Sr3NiIrO6 play no role in
determining the Ir spin conﬁguration.
In summary, we combined infrared and optical spectroscopy with high-ﬁeld magnetization and ﬁrst-principles calculations to explore coupling processes involving the fundamental excitations of the lattice in Sr3NiIrO6—a material with signiﬁcant spin–orbit
interactions. These include both spin–lattice and electron–phonon processes. Magneto-infrared spectroscopy reveals that three phonons—all of which modulate the magnetic pathways around and the symmetry of the Ir centers—display strong spin–lattice interactions, demonstrating that the approach to the coerciveﬁeld takes place with very speciﬁc local lattice distortions—different from expectations for simple domain reorientation in a ferro-magnet. Examination of the mode displacement patterns also provides a speciﬁc mechanism for inter-chain interactions, a
ﬁnding that is crucial to the development of the working magnetic model in Sr3NiIrO6 and related materials. At the same time,
analysis of the on-site Ir4+ excitations unveils vibronic coupling and extremely large crystalﬁeld parameters. For instance, 10Dqis a factor of two larger than that in traditional transition metal oxides, and the Racah parameter B is a factor of 10 higher. Moreover, the phonon that activates the vibronic coupling has a completely different displacement pattern than those that are sensitive to magneticﬁeld. We thereforeﬁnd that certain phonons in Sr3NiIrO6 are strongly entangled with the spin and charge
channels. In addition, the diffuse character of the Ir 5dorbitals determines the ground-state spin structure of Sr3NiIrO6, whereas
spin–lattice interactions reduce the energy required to modify microscopic spin arrangements. Returning to the developing magnetic model of Sr3NiIrO6, we qualitatively expect that the
ultra-high coerciveﬁeld results from the high barrier toﬂipping a chain of strongly coupled Ni2+and Ir4+magnetic moments, which is effectively a many-body magnetic system. This barrier to
ﬂipping results from the interaction of the magnetic order with the lattice. This interaction has two parts: the interaction of the magnetic exchange interactions with lattice distortions and the mixing of the local spin–orbit coupled state of the Ir4+ion
with the lattice. We quantiﬁed both in this work, thereby providing necessary insight to develop a complete model.
High-quality single crystals were grown as described previously18,57and either polished or combined with a transparent matrix to control optical density due to strong phonon absorption. Absorption was calculated as
hdlnðT ðωÞÞ, wherehis concentration,dis thickness, andT ðωÞis the measured transmittance. Magneto-infrared and magnetization measure-ments were carried out at the National High Magnetic Field Laboratory using the 35 T resistive and 65 T short-pulse magnets, respectively. Absorption was obtained at zeroﬁeld, and magneto-infrared measure-ments tracked changes. Absorption differences were calculated asΔα=α (B)−α(0 T). We integrated |Δα| over small energy windows (127–150, 290–335, and 530–545 cm−1) to quantify changes and renormalize to the 35 T magnetization squared to match energy scales and provide a proper comparison.
First-principles calculations were performed using projector-augmented waves as implemented in VASP.58,59 The PBEsol functional was used to
approximate the exchange correlation energy,60,61and density functional theory+U62 was utilized for the transition metals. For calculations of
Sr3NiIrO6,U=5 eV for Ni andU=1 eV for Ir were used. For the Cu analog,
U=5 eV for Cu andU=1.5 for Ir were used. Changing the values ofUand
J changes the obtained phonon frequencies but does not affect the physical picture. Phonons were calculated using both the direct method and density functional perturbation theory, and the results were identical within numerical noise. An 8 × 8 × 8 Monkhorst–Pack grid63and a plane wave energy cutoff of 500 eV gave good convergence. The crystal structure used in the phonon calculations was obtained by relaxing the experimentally reported structure in the magnetically ordered phase.
The complexity of the crystal and magnetic structure of Sr3NiIrO6makes
it impractical to perform a detailed ﬁrst-principles calculation of the spin–phonon or spin–lattice coupling in this material. In order to gain insight about the spin–lattice coupling strength, we therefore performed noncollinear magnetic calculations in a series of crystal structures that were obtained by displacing the atoms according to the displacement pattern of particular phonon modes. (Results are presented in Fig.1j.) We considered displacements up to 0.5 Å in total for the 22 atom unit cell, which corresponds to an average of ~0.1 Å per atom. The magnetic ground state does not change and is still predominantly ferrimagnetic along thec
axis for all of these structures. However, unlike the collinear ferrimagnetic state observed in the experiment and reproduced by ﬁrst-principles calculations, the magnetic ground state for these displaced structures are tilted ferrimagnetic. The 310 cm−1displacement gives rise to large tilting
of Ni moments—as much as ≈10° for the larger displacements we considered. For reference, we also present the results of the same calculation for the 177 cm−1mode of same symmetry andﬁnd a much smaller tilting. This observation is not surprising, because the character of this mode does not change the exchange pathways signiﬁcantly. (It is of 49% Sr, 13% Ni, 8% Ir, and only 29% O character.) Thisﬁnding is also in line with the experimental result that this mode is not engaged in spin–lattice coupling.
Data are available from the corresponding author upon reasonable request.
Research at the University of Tennessee, Rutgers University, and University of Minnesota is supported by the National Science Foundation DMREF program (DMR-1629079, DMR-1629059, and DMR-1629260, respectively). The crystal growth was partially supported by the National Research Foundation of Korea (NRF) funded by the Ministry of Science and ICT (No. 2016K1A4A4A01922028). We also appreciate funding from the U.S. Department of Energy, Basic Energy Sciences, contract DE-FG02-01ER45885 (Tennessee),“Science at 100 Tesla”(LANL), and“Topological phases of quantum matter and decoherence”(LANL). The NHMFL facility is supported by the U.S. National Science Foundation through Cooperative Grant DMR-1644779, the State of Florida, and the U.S. Department of Energy. We appreciate useful conversations with Brian J. Donahue.
J.L.M., T.B. and S.-W.C. devised the project. X.L. and S.-W.C. grew the samples. K.R.O., A.A.W., K.D.H., A.L.B., M.O. and J.L.M. carried out the spectroscopic measurements. V.S.Z., C.V.T. and J.S. measured the magnetic properties. A.P. and T.B. performed the theoretical calculations. K.R.O., J.L.M., V.S.Z. and T.B. wrote the manuscript, and all authors contributed to it.
Supplementary Informationaccompanies the paper on thenpj Quantum Materials website (https://doi.org/10.1038/s41535-019-0184-x).
Competing interests:The authors declare no competing interests.
Publisher’s note:Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations.
1. Rau, J. G., Lee, E. K.-H. & Kee, H.-Y. Spin-orbit physics giving rise to novel phases in correlated systems: iridates and related materials.Annu. Rev. Condens. Matter Phys.7, 195–221 (2016).
2. Witczak-Krempa, W., Chen, G., Kim, Y. B. & Balents, L. Correlated quantum phe-nomena in the strong spin-orbit regime.Annu. Rev. Condens. Matter Phys.5, 57–82 (2014).
3. Feng, H. L. et al. High-temperature ferrimagnetism with large coercivity and exchange bias in the partially ordered 3d/5d hexagonal perovskite Ba2Fe1.12Os0.88O6.Chem. Mater.29, 886–895 (2017).
4. Feng, H. L. et al. Canted ferrimagnetism and giant coercivity in the non-stoichiometric double perovskite La2Ni1.19Os0.81O6.Phys. Rev. B97, 184407 (2018).
6. Isobe, M., Kimoto, K., Arai, M. & Takayama-Muromachi, E. Superconductivity in BaIrSi2: A 5delectron system with a noncentrosymmetric crystal structure.Phys. Rev. B99, 054514 (2019).
7. Cao, G. et al. Electrical control of structural and physical properties via strong spin-orbit interactions in Sr2IrO4.Phys. Rev. Lett.120, 017201 (2018).
8. Kim, B. J. et al. Phase-sensitive observation of a spin-orbital Mott state in Sr2IrO4. Science323, 1329–1332 (2009).
9. Clancy, J. P. et al. Pressure-driven collapse of the relativistic electronic ground state in a honeycomb iridate.npj Quantum Mater.3, 35 (2018).
10. Yang, J. J. et al. Charge-orbital density wave and superconductivity in the strong spin-orbit coupled IrTe2:Pd.Phys. Rev. Lett.108, 116402 (2012).
11. Hsu, P.-J. et al. Hysteretic melting transition of a soliton lattice in a commensurate charge modulation.Phys. Rev. Lett.111, 266401 (2013).
12. Zheng, F., Tan, L. Z., Liu, S. & Rappe, A. M. Rashba spin-orbit coupling enhanced carrier lifetime in CH3NH3PbI3.Nano Lett.15, 7794–7800 (2015).
13. Goldman, N., Beugeling, W. & Smith, C. M. Topological phase transitions between chiral and helical spin textures in a lattice with spin-orbit coupling and a mag-neticﬁeld.Europhys. Lett.97, 23003 (2012).
14. Bihlmayer, G., Blügel, S. & Chulkov, E. V. Enhanced Rashba spin-orbit splitting in Bi/Ag (111) and Pb/Ag (111) surface alloys fromﬁrst principles.Phys. Rev. B75, 195414 (2007).
15. Sie, E. J. et al. An ultrafast symmetry switch in a Weyl semimetal.Nature565, 61–66 (2019).
16. Charnukha, A. et al. Correlation-driven metal-insulator transition in proximity to an iron-based superconductor.Phys. Rev. B96, 195121 (2017).
17. Liu, Z.-H. et al. Reduced electronic correlation effects in half substituted Ba(Fe1−xCox)2As2.Appl. Phys. Lett.112, 232602 (2018).
18. Singleton, J. et al. Magnetic properties of Sr3NiIrO6 and Sr3CoIrO6: magnetic
hysteresis with coerciveﬁelds of up to 55 T.Phys. Rev. B94, 224408 (2016). 19. Ristau, R. A., Barmak, K., Lewis, L. H., Coffey, K. R. & Howard, J. K. On the
rela-tionship of high coercivity andL10ordered phase in CoPt and FePt thinﬁlms.J. Appl. Phys.86, 4527–4533 (1999).
20. Bai, G., Gao, R. W., Sun, Y., Han, G. B. & Wang, B. Study of high-coercivity sintered NdFeB magnets.J. Magn. Magn. Mater.308, 20–23 (2007).
21. Wu, W. et al. Formation of pancakelike Ising domains and giant magnetic coer-civity in ferrimagnetic LuFe2O4.Phys. Rev. Lett.101, 137203 (2008).
22. Ou, X. & Wu, H. Impact of spin-orbit coupling on the magnetism of Sr3MIrO6(M=
Ni, Co).Sci. Rep.4, 4609 (2014).
23. Zhang, G. R., Zhang, X. L., Jia, T., Zeng, Z. & Lin, H. Q. Intrachain antiferromagnetic interaction and Mott state induced by spin-orbit coupling in Sr3NiIrO6.J. Appl. Phys.107, 09E120 (2010).
24. Birol, T., Haule, K. & Vanderbilt, D. Nature of the magnetic interactions in Sr3NiIrO6.Phys. Rev. B98, 134432 (2018).
25. Mikhailova, D. et al. Magnetic properties and crystal structure of Sr3CoIrO6and
Sr3NiIrO6.Phys. Rev. B86, 134409 (2012).
26. Lefrançois, E. et al. Magnetic order in the frustrated Ising-like chain compound Sr3NiIrO6.Phys. Rev. B90, 014408 (2014).
27. Toth, S., Wu, W., Adroja, D. T., Rayaprol, S. & Sampathkumaran, E. V. Frustrated Ising chains on the triangular lattice in Sr3NiIrO6.Phys. Rev. B93, 174422 (2016).
28. Lefrançois, E. et al. Anisotropic interactions opposing magnetocrystalline aniso-tropy in Sr3NiIrO6.Phys. Rev. B93, 224401 (2016).
29. Stitzer, K. E., Henley, W. H., Claridge, J. B., zur Loye, H. C. & Layland, R. C. Sr3NiRhO6
and Sr3CuRhO6- two new one-dimensional oxides. Magnetic behavior as a
function of structure: commensurate vs incommensurate.J. Solid State Chem. 164, 220–229 (2002).
30. Niitaka, S., Yoshimura, K., Kosuge, K., Nishi, M. & Kakurai, K. Partially disordered antiferromagnetic phase in Ca3CoRhO6.Phys. Rev. Lett.87, 177202 (2001).
31. Mohapatra, N., Iyer, K. K., Rayaprol, S. & Sampathkumaran, E. V. Geometrically frustrated magnetic behavior of Sr3NiRhO6and Sr3NiPtO6.Phys. Rev. B75, 214422
32. Murthy, J. K., Nileena, N., Vishnugopal, V. S. & Anil Kumar, P. S. Partially-disordered to frozen-state crossover induced magnetocaloric properties of the anti-ferromagnetic one-dimensional spin-chain Sr3CoIrO6. Mater. Res. Express 6,
33. Brinzari, T. V. et al. Magnetoelastic coupling in [Ru2(O2CMe)4]3[Cr(CN)6]
molecule-based magnet.Phys. Rev. B86, 214411 (2012).
34. Granado, E. et al. Magnetic ordering effects in the Raman spectra of La1−xMn1−xO3. Phys. Rev. B60, 11879–11882 (1999).
35. Poirier, M., Laliberté, F., Pinsard-Gaudart, L. & Revcolevschi, A. Magnetoelastic coupling in hexagonal multiferroic YMnO3using ultrasound measurements.Phys. Rev. B76, 174426 (2007).
36. Poirier, M., Lemyre, J. C., Lahaie, P.-O., Pinsard-Gaudart, L. & Revcolevschi, A. Enhanced magnetoelastic coupling in hexagonal multiferroic HoMnO3.Phys. Rev. B83, 054418 (2011).
37. Casto, L. D. et al. Strong spin-lattice coupling in CrSiTe3.APL Mater.3, 041515 (2015).
38. Yokosuk, M. O. et al. Tracking the continuous spin-ﬂop transition in Ni3TeO6by
infrared spectroscopy.Phys. Rev. B92, 144305 (2015).
39. Kim, J. W. et al. Successive magnetic-ﬁeld-induced transitions and colossal magnetoelectric effect in Ni3TeO6.Phys. Rev. Lett.115, 137201 (2015).
40. Jaime, M. et al. Magnetostriction and magnetic texture up to 100.75 Tesla in frustrated SrCu2(BO3)2.Proc. Natl Acad. Sci.109, 12404–12407 (2012).
41. Liu, X. et al. Testing the validity of the strong spin-orbit-coupling limit for octa-hedrally coordinated iridate compounds in a model system Sr3CuIrO6.Phys. Rev. Lett.109, 157401 (2012).
42. Sell, D. D., Greene, R. L. & White, R. M. Optical exciton-magnon absorption in MnF2.Phys. Rev.158, 489–510 (1967).
43. Lohr, L. L. Jr. Spin-forbidden electronic excitations in transition metal complexes. Coord. Chem. Rev.8, 241–259 (1972).
44. Ballhausen, C. J.Introduction to Ligand Field Thoery(McGraw-Hill, New York, 1962). 45. O’Neal, K. R. et al. Vibronic coupling and band gap trends in CuGeO3nanorods.
Phys. Rev. B96, 075437 (2017).
46. Park, H. J. et al. Phonon-assisted optical excitation in the narrow bandgap Mott insulator Sr3Ir2O7.Phys. Rev. B89, 155115 (2014).
47. Flahaut, D. et al. A magnetic study of the one dimensional Sr3NiIrO6compound. Eur. Phys. J. B35, 317–323 (2003).
48. Tanabe, Y. & Sugano, S. On the absorption spectra of complex ions. I.J. Phys. Soc. Jpn.9, 753–766 (1954).
49. Tanabe, Y. & Sugano, S. On the absorption spectra of compex ions II.J. Phys. Soc. Jpn.9, 766–779 (1954).
50. Tanabe, Y. & Sugano, S. On the absorption spectra of complex ions, III The calculation of the crystallineﬁeld strength.J. Phys. Soc. Jpn.11, 864–877 (1956). 51. Sala, M. M. et al. Crystalﬁeld splitting in Srn+1IrnO3n+1(n=1,2) iridates probed by
x-ray Raman spectroscopy.Phys. Rev. B90, 085126 (2014).
52. Ishii, K. et al. Momentum-resolved electronic excitations in the Mott insulator Sr2IrO4studied by resonant inelastic x-ray scattering.Phys. Rev. B83, 115121
53. Gretarsson, H. et al. Crystal-ﬁeld splitting and correlation effect on the electronic structure ofA2IrO3.Phys. Rev. Lett.110, 076402 (2013).
54. Marusak, L. A., Messier, R. & White, W. B. Optical absorption spectrum of hematite, αFe2O3near IR to UV.J. Phys. Chem. Solids41, 981–984 (1980).
55. Yokosuk, M. O. et al. Magnetoelectric coupling through the spinﬂop transition in Ni3TeO6.Phys. Rev. Lett.117, 147402 (2016).
56. Ma, C.-G. & Brik, M. G. Systematic analysis of spectroscopic characteristics of heavy transition metal ions with 4dN
(N=1…10) electronic conﬁ gura-tions in a free state.J. Lumin.145, 402–409 (2014).
57. Nguyen, T. N. & zur Loye, H.-C. A family of one-dimensional oxides: Sr3MIrO6(M=
Ni, Cu, Zn): Structure and magnetic properties.J. Solid State Chem.117, 300–308 (1995).
58. Kresse, G. & Furthmüller, J. Efﬁcient iterative schemes forab initiototal-energy calculations using a plane-wave basis set.Phys. Rev. B54, 11169–11186 (1996). 59. Kresse, G. & Furthmüller, J. Efﬁciency of ab-initio total energy calculations for
metals and semiconductors using a plane-wave basis set.Comput. Mater. Sci.6, 15–50 (1996).
60. Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple.Phys. Rev. Lett.77, 3865–3868 (1996).
61. Perdew, J. P. et al. Generalized gradient approximation for solids and their sur-faces.Phys. Rev. Lett.100, 136406 (2008).
62. Liechtenstein, A. I., Anisimov, V. I. & Zaanen, J. Density-functional theory and strong interactions: orbital ordering in Mott-Hubbard insulators.Phys. Rev. B52, 5467–5471 (1995).
63. Monkhorst, H. J. & Pack, J. D. Special points for Brillouin-zone integrations.Phys. Rev. B13, 5188–5192 (1976).
Open AccessThis article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visithttp://creativecommons. org/licenses/by/4.0/.